# Electronic Supplementary Material (ESI) for Green Chemistry.
# This journal is © The Royal Society of Chemistry 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_BWCu
_database_code_depnum_ccdc_archive 'CCDC 2052783'
loop_
_audit_author_name
_audit_author_address
'Shenzhen Chang'
;Dalian University of Technology
China
;
_audit_update_record             
;
2021-06-15 deposited with the CCDC.	2021-09-29 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2018/3
_shelx_SHELXL_version_number     2018/3
_chemical_name_systematic        BWCu
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C18 H48 B Cu3 K3 N24 O66 W12'
_chemical_formula_weight         4181.73

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      trigonal
_space_group_IT_number           148
_space_group_name_H-M_alt        'R -3 :H'
_space_group_name_Hall           '-R 3'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'

_cell_length_a                   35.1668(9)
_cell_length_b                   35.1668(9)
_cell_length_c                   20.2270(6)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     21663.5(12)
_cell_formula_units_Z            9
_cell_measurement_temperature    190(2)
_cell_measurement_reflns_used    8468
_cell_measurement_theta_min      2.317
_cell_measurement_theta_max      24.994

_exptl_crystal_description       Strip
_exptl_crystal_colour            blue
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.885
_exptl_crystal_F_000             17001
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.270
_exptl_crystal_size_mid          0.150
_exptl_crystal_size_min          0.150
_exptl_absorpt_coefficient_mu    15.153
_shelx_estimated_absorpt_T_min   0.105
_shelx_estimated_absorpt_T_max   0.210
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.082
_exptl_absorpt_correction_T_max  0.103
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      190(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            39054
_diffrn_reflns_av_unetI/netI     0.0392
_diffrn_reflns_av_R_equivalents  0.0503
_diffrn_reflns_limit_h_min       -41
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_k_min       -41
_diffrn_reflns_limit_k_max       41
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_theta_min         2.317
_diffrn_reflns_theta_max         24.994
_diffrn_reflns_theta_full        24.994
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             8468
_reflns_number_gt                8059
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          
;
Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0001P)²+4304.4702P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         8468
_refine_ls_number_parameters     646
_refine_ls_number_restraints     111
_refine_ls_R_factor_all          0.0808
_refine_ls_R_factor_gt           0.0775
_refine_ls_wR_factor_ref         0.1667
_refine_ls_wR_factor_gt          0.1653
_refine_ls_goodness_of_fit_ref   1.350
_refine_ls_restrained_S_all      1.345
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
B1 B 0.500000 0.000000 1.000000 0.059(12) Uani 1 2 d S U P . .
W1 W 0.51678(3) 0.01073(3) 0.82963(4) 0.0264(2) Uani 1 1 d . . . . .
W2 W 0.49145(3) 0.08032(3) 1.08797(5) 0.0355(2) Uani 1 1 d . . . . .
W3 W 0.41518(3) -0.01453(3) 0.89506(4) 0.0335(2) Uani 1 1 d . . . . .
W4 W 0.60038(3) 0.02272(3) 0.93501(5) 0.0364(2) Uani 1 1 d . . . . .
W5 W 0.50579(3) 0.08964(3) 0.91776(5) 0.0350(2) Uani 1 1 d . . . . .
W6 W 0.59170(3) 0.10407(3) 1.02043(5) 0.0434(3) Uani 1 1 d . . . . .
Cu1 Cu 0.76124(10) 0.01409(9) 1.03153(14) 0.0359(6) Uani 1 1 d . . . . .
K2 K 0.4948(4) -0.2330(4) 1.0235(8) 0.043(3) Uani 0.5 1 d . . P A 1
Cu2 Cu 0.4991(3) -0.2337(2) 0.9799(5) 0.053(2) Uani 0.5 1 d . . P A 2
K1 K 0.6523(2) -0.04061(18) 0.8593(3) 0.0460(13) Uani 1 1 d . . . . .
O1 O 0.4892(8) 0.0133(9) 0.9360(12) 0.022(6) Uani 0.5 1 d . . P . .
O2 O 0.5510(9) 0.0250(9) 1.0129(12) 0.025(6) Uani 0.5 1 d . . P . .
O3 O 0.5144(9) 0.0503(9) 1.0026(14) 0.028(6) Uani 0.5 1 d . . P . .
O4 O 0.5208(9) -0.0090(10) 0.9421(14) 0.029(7) Uani 0.5 1 d . . P . .
O5 O 0.8044(6) 0.0424(5) 0.9614(8) 0.046(4) Uani 1 1 d . . . . .
O6 O 0.6850(6) -0.0549(7) 0.9815(9) 0.058(5) Uani 1 1 d . . . . .
O7 O 0.7651(9) 0.1880(8) 1.0407(12) 0.090(7) Uani 1 1 d . U . . .
H7A H 0.775169 0.213465 1.056110 0.135 Uiso 1 1 calc R U . . .
O8 O 0.4899(9) 0.1093(10) 1.0010(13) 0.021(6) Uani 0.5 1 d . U P . .
O8A O 0.4846(10) 0.0863(10) 1.0034(14) 0.024(6) Uani 0.5 1 d . U P . .
O9 O 0.8457(7) 0.1015(8) 1.0149(11) 0.083(7) Uani 1 1 d . U . . .
O10 O 0.7063(5) -0.0248(5) 1.0792(7) 0.037(4) Uani 1 1 d . . . . .
O11 O 0.7413(6) 0.2136(6) 0.9590(11) 0.058(5) Uani 1 1 d . . . . .
O12 O 0.6482(5) 0.0328(6) 0.9023(8) 0.047(4) Uani 1 1 d . . . . .
O13 O 0.4875(6) 0.1184(6) 1.1336(8) 0.048(4) Uani 1 1 d . . . . .
O14 O 0.3750(5) -0.0212(6) 0.8445(8) 0.045(4) Uani 1 1 d . . . . .
O15 O 0.5089(7) 0.1331(6) 0.8769(10) 0.062(6) Uani 1 1 d . . . . .
O16 O 0.5240(6) 0.0656(6) 0.8489(11) 0.062(6) Uani 1 1 d . . . . .
O17 O 0.6369(6) 0.1527(5) 1.0293(9) 0.048(4) Uani 1 1 d . . . . .
O18 O 0.4474(6) 0.0481(6) 0.8972(11) 0.058(5) Uani 1 1 d . . . . .
O19 O 0.4551(6) -0.0131(6) 0.8310(10) 0.055(5) Uani 1 1 d . . . . .
O20 O 0.5243(7) 0.0145(6) 0.7464(8) 0.070(7) Uani 1 1 d . . . . .
O21 O 0.6006(9) 0.0737(6) 1.0864(8) 0.077(8) Uani 1 1 d . . . . .
O22 O 0.5047(6) -0.0472(6) 0.8410(13) 0.075(7) Uani 1 1 d . . . . .
O23 O 0.5744(6) 0.0307(6) 0.8575(12) 0.069(7) Uani 1 1 d . . . . .
O24 O 0.5551(9) 0.1191(10) 1.0799(14) 0.023(6) Uani 0.5 1 d . U P . .
O24A O 0.5494(11) 0.0960(11) 1.0779(15) 0.032(7) Uani 0.5 1 d . U P . .
O25 O 0.5701(7) -0.0379(7) 0.9173(11) 0.068(6) Uani 1 1 d . U . . .
O26 O 0.6129(9) 0.0794(8) 0.9576(11) 0.081(7) Uani 1 1 d . U . . .
O27 O 0.4033(11) -0.0075(11) 0.9791(16) 0.033(7) Uani 0.5 1 d . U P . .
O27A O 0.3790(11) -0.0162(10) 0.9738(15) 0.031(7) Uani 0.5 1 d . U P . .
O28 O 0.5667(9) 0.1268(10) 0.9502(13) 0.021(6) Uani 0.5 1 d . U P . .
O28A O 0.5613(9) 0.1028(10) 0.9495(14) 0.024(6) Uani 0.5 1 d . U P . .
O1W O 0.7870(6) 0.0399(6) 1.1325(8) 0.049(4) Uani 1 1 d . . . . .
O2W O 0.6999(15) -0.0864(4) 0.8661(16) 0.20(2) Uani 1 1 d D U . . .
O3W O 0.4647(15) -0.2932(16) 0.937(2) 0.077(13) Uani 0.5 1 d . U P . .
O4W O 0.457(2) -0.238(2) 1.066(3) 0.105(18) Uani 0.5 1 d . U P . .
O5W O 0.4741(15) -0.2159(15) 0.904(2) 0.070(12) Uani 0.5 1 d . U P . .
O6W O 0.5119(18) -0.1988(18) 1.165(3) 0.100(16) Uani 0.5 1 d . U P . .
OW1 O 0.666667 -0.166667 0.833333 0.023(4) Uiso 1 2 d DS . P . .
OW2 O 0.7339(17) -0.1422(17) 0.830(2) 0.084(14) Uiso 0.5 1 d . . P . .
OW3 O 0.6672(14) -0.1448(11) 0.9564(7) 0.072(12) Uiso 0.5 1 d D . P . .
OW4 O 0.6607(14) -0.1821(14) 0.927(2) 0.067(11) Uiso 0.5 1 d . . P . .
OW5 O 0.7808(11) -0.0131(11) 0.8491(17) 0.127(11) Uiso 1 1 d . . . . .
N1 N 0.5988(6) -0.1088(6) 1.0276(9) 0.035(4) Uani 1 1 d . . . . .
N2 N 0.7403(7) 0.0564(6) 1.0180(9) 0.036(4) Uani 1 1 d . . . . .
N3 N 0.9169(6) 0.1267(6) 0.9334(11) 0.042(5) Uani 1 1 d . . . . .
N4 N 0.9710(6) 0.1894(7) 0.9574(10) 0.039(5) Uani 1 1 d . . . . .
N5 N 0.7265(6) 0.1071(7) 0.9858(9) 0.040(5) Uani 1 1 d . . . . .
N6 N 0.7144(8) 0.0618(8) 1.0631(11) 0.053(6) Uani 1 1 d . . . . .
N7 N 0.7065(8) 0.0912(7) 1.0464(10) 0.052(6) Uani 1 1 d . . . . .
N8 N 0.5469(8) -0.1736(8) 1.0004(15) 0.062(8) Uani 1 1 d . . . . .
N9 N 0.9514(9) 0.1217(8) 0.9351(18) 0.086(10) Uani 1 1 d . . . . .
N10 N 0.5637(8) -0.1475(9) 0.9464(16) 0.069(8) Uani 1 1 d . . . . .
N11 N 0.9840(9) 0.1588(10) 0.9496(16) 0.081(9) Uani 1 1 d . . . . .
N12 N 0.5958(7) -0.1091(7) 0.9603(11) 0.047(5) Uani 1 1 d . . . . .
C1 C 0.5685(10) -0.1470(11) 1.0510(17) 0.066(9) Uani 1 1 d . . . . .
C2 C 0.7441(10) 0.1844(8) 0.9866(16) 0.054(7) Uani 1 1 d . . . . .
C3 C 0.9302(9) 0.1665(9) 0.9480(12) 0.045(6) Uani 1 1 d . . . . .
H3A H 0.910978 0.178112 0.951603 0.055 Uiso 1 1 calc R U . . .
C4 C 0.8736(8) 0.0896(7) 0.9167(14) 0.045(6) Uani 1 1 d . . . . .
H4A H 0.876772 0.063657 0.907417 0.054 Uiso 1 1 calc R U . . .
H4B H 0.863221 0.096756 0.875598 0.054 Uiso 1 1 calc R U . . .
C5 C 0.7474(7) 0.0845(7) 0.9708(10) 0.032(5) Uani 1 1 d . . . . .
H5A H 0.764410 0.088565 0.932264 0.038 Uiso 1 1 calc R U . . .
C6 C 0.7234(9) 0.1410(7) 0.9511(13) 0.044(6) Uani 1 1 d . . . . .
H6A H 0.692052 0.131105 0.943276 0.053 Uiso 1 1 calc R U . . .
H6B H 0.737716 0.145311 0.907383 0.053 Uiso 1 1 calc R U . . .
C7 C 0.8396(9) 0.0776(9) 0.9685(13) 0.049(7) Uani 1 1 d . . . . .
C8 C 0.6761(7) -0.0496(7) 1.0366(11) 0.032(5) Uani 1 1 d . . . . .
C9 C 0.6298(8) -0.0689(8) 1.0629(15) 0.050(7) Uani 1 1 d . . . . .
H9A H 0.629486 -0.075834 1.110401 0.060 Uiso 1 1 calc R U . . .
H9B H 0.620254 -0.046907 1.058760 0.060 Uiso 1 1 calc R U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
B1 O1 1.49(2) 10_657 ?
B1 O1 1.49(2) . ?
B1 O4 1.50(3) . ?
B1 O4 1.50(3) 10_657 ?
B1 O2 1.58(3) 10_657 ?
B1 O2 1.58(3) . ?
B1 O3 1.58(3) 10_657 ?
B1 O3 1.58(3) . ?
W1 O20 1.699(16) . ?
W1 O16 1.858(18) . ?
W1 O23 1.869(16) . ?
W1 O22 1.876(18) . ?
W1 O19 1.894(17) . ?
W1 O1 2.38(2) . ?
W1 O4 2.40(3) . ?
W2 O13 1.689(15) . ?
W2 O8A 1.76(3) . ?
W2 O24A 1.84(3) . ?
W2 O22 1.90(2) 10_657 ?
W2 O25 1.92(2) 10_657 ?
W2 O24 1.96(3) . ?
W2 O8 2.05(3) . ?
W2 O3 2.37(3) . ?
W2 O4 2.40(3) 10_657 ?
W3 O14 1.663(14) . ?
W3 O27 1.80(3) . ?
W3 O19 1.894(18) . ?
W3 O21 1.903(17) 10_657 ?
W3 O18 1.907(18) . ?
W3 O27A 2.02(3) . ?
W3 O2 2.33(2) 10_657 ?
W3 O1 2.42(2) . ?
W4 O12 1.672(16) . ?
W4 O27 1.80(3) 10_657 ?
W4 O26 1.87(2) . ?
W4 O25 1.88(2) . ?
W4 O23 1.90(2) . ?
W4 O27A 2.04(3) 10_657 ?
W4 O2 2.38(3) . ?
W4 O4 2.44(3) . ?
W4 K1 3.835(6) . ?
W5 O15 1.694(17) . ?
W5 O8A 1.87(3) . ?
W5 O18 1.878(18) . ?
W5 O28A 1.88(3) . ?
W5 O16 1.899(18) . ?
W5 O28 1.98(3) . ?
W5 O8 2.00(3) . ?
W5 O3 2.32(3) . ?
W5 O1 2.47(3) . ?
W6 O17 1.662(17) . ?
W6 O28A 1.78(3) . ?
W6 O24A 1.79(3) . ?
W6 O21 1.83(2) . ?
W6 O26 1.89(2) . ?
W6 O24 2.02(3) . ?
W6 O28 2.03(3) . ?
W6 O2 2.41(3) . ?
W6 O3 2.44(3) . ?
Cu1 O5 1.948(16) . ?
Cu1 O10 1.972(16) . ?
Cu1 N2 1.981(19) . ?
Cu1 N4 1.99(2) 12_547 ?
Cu1 O1W 2.235(17) . ?
Cu1 K1 3.901(6) 5_545 ?
K2 O4W 1.51(6) . ?
K2 O11 1.82(2) 12_547 ?
K2 N8 2.03(3) . ?
K2 O3W 2.54(5) . ?
K2 O5W 2.67(4) . ?
K2 C2 2.78(3) 12_547 ?
K2 C1 2.89(4) . ?
K2 O6W 3.05(6) . ?
K2 N10 3.17(3) . ?
K2 O7 3.20(3) 12_547 ?
Cu2 N8 1.98(2) . ?
Cu2 O5W 2.01(4) . ?
Cu2 O3W 2.02(5) . ?
Cu2 O11 2.05(2) 12_547 ?
Cu2 O4W 2.23(6) . ?
K1 O12 2.79(2) . ?
K1 O2W 2.85(4) . ?
K1 N6 2.86(2) 9_654 ?
K1 O1W 2.868(18) 9_654 ?
K1 O6 2.88(2) . ?
K1 O10 2.904(16) 9_654 ?
K1 O14 2.908(16) 18_546 ?
K1 N12 3.02(2) . ?
K1 O25 3.16(2) . ?
O1 O4 1.65(4) . ?
O1 O2 1.73(4) 10_657 ?
O1 O3 1.77(4) . ?
O3 O4 1.76(4) 10_657 ?
O5 C7 1.25(3) . ?
O6 C8 1.20(3) . ?
O7 C2 1.29(4) . ?
O8 O8A 0.74(3) . ?
O9 C7 1.21(3) . ?
O10 C8 1.30(3) . ?
O11 C2 1.21(3) . ?
O24 O24A 0.74(3) . ?
O27 O27A 0.76(3) . ?
O28 O28A 0.76(3) . ?
OW3 OW4 1.35(5) . ?
N1 C1 1.32(3) . ?
N1 N12 1.37(3) . ?
N1 C9 1.46(3) . ?
N2 C5 1.31(3) . ?
N2 N6 1.37(3) . ?
N3 C3 1.27(3) . ?
N3 N9 1.31(3) . ?
N3 C4 1.47(3) . ?
N4 C3 1.26(3) . ?
N4 N11 1.37(3) . ?
N5 C5 1.36(3) . ?
N5 N7 1.38(3) . ?
N5 C6 1.44(3) . ?
N6 N7 1.25(3) . ?
N8 C1 1.34(4) . ?
N8 N10 1.36(4) . ?
N9 N11 1.27(4) . ?
N10 N12 1.29(3) . ?
C2 C6 1.51(3) . ?
C4 C7 1.48(4) . ?
C8 C9 1.51(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 B1 O1 180.0 10_657 . ?
O1 B1 O4 112.7(15) 10_657 . ?
O1 B1 O4 67.3(15) . . ?
O1 B1 O4 67.3(15) 10_657 10_657 ?
O1 B1 O4 112.7(15) . 10_657 ?
O4 B1 O4 180.0 . 10_657 ?
O1 B1 O2 111.5(13) 10_657 10_657 ?
O1 B1 O2 68.5(13) . 10_657 ?
O4 B1 O2 107.0(14) . 10_657 ?
O4 B1 O2 73.0(14) 10_657 10_657 ?
O1 B1 O2 68.5(13) 10_657 . ?
O1 B1 O2 111.5(13) . . ?
O4 B1 O2 73.0(14) . . ?
O4 B1 O2 107.0(14) 10_657 . ?
O2 B1 O2 180.0 10_657 . ?
O1 B1 O3 70.5(14) 10_657 10_657 ?
O1 B1 O3 109.5(14) . 10_657 ?
O4 B1 O3 69.8(15) . 10_657 ?
O4 B1 O3 110.2(15) 10_657 10_657 ?
O2 B1 O3 74.4(14) 10_657 10_657 ?
O2 B1 O3 105.6(14) . 10_657 ?
O1 B1 O3 109.5(14) 10_657 . ?
O1 B1 O3 70.5(14) . . ?
O4 B1 O3 110.2(15) . . ?
O4 B1 O3 69.8(15) 10_657 . ?
O2 B1 O3 105.6(14) 10_657 . ?
O2 B1 O3 74.4(14) . . ?
O3 B1 O3 180.0 10_657 . ?
O20 W1 O16 101.0(10) . . ?
O20 W1 O23 100.0(11) . . ?
O16 W1 O23 89.3(9) . . ?
O20 W1 O22 98.5(11) . . ?
O16 W1 O22 160.4(11) . . ?
O23 W1 O22 89.1(8) . . ?
O20 W1 O19 98.4(10) . . ?
O16 W1 O19 89.3(8) . . ?
O23 W1 O19 161.4(10) . . ?
O22 W1 O19 86.1(8) . . ?
O20 W1 O1 160.5(11) . . ?
O16 W1 O1 67.5(9) . . ?
O23 W1 O1 95.7(10) . . ?
O22 W1 O1 93.2(11) . . ?
O19 W1 O1 66.8(8) . . ?
O20 W1 O4 158.7(11) . . ?
O16 W1 O4 96.0(10) . . ?
O23 W1 O4 67.2(10) . . ?
O22 W1 O4 65.5(11) . . ?
O19 W1 O4 94.5(9) . . ?
O1 W1 O4 40.5(9) . . ?
O13 W2 O8A 111.5(11) . . ?
O13 W2 O24A 109.9(12) . . ?
O8A W2 O24A 93.1(14) . . ?
O13 W2 O22 97.6(10) . 10_657 ?
O8A W2 O22 150.3(12) . 10_657 ?
O24A W2 O22 81.9(12) . 10_657 ?
O13 W2 O25 98.0(10) . 10_657 ?
O8A W2 O25 82.5(12) . 10_657 ?
O24A W2 O25 151.2(13) . 10_657 ?
O22 W2 O25 87.9(8) 10_657 10_657 ?
O13 W2 O24 90.6(11) . . ?
O8A W2 O24 90.7(13) . . ?
O24A W2 O24 22.0(10) . . ?
O22 W2 O24 94.8(10) 10_657 . ?
O25 W2 O24 170.5(11) 10_657 . ?
O13 W2 O8 92.3(10) . . ?
O8A W2 O8 20.5(10) . . ?
O24A W2 O8 93.3(13) . . ?
O22 W2 O8 169.9(12) 10_657 . ?
O25 W2 O8 92.2(10) 10_657 . ?
O24 W2 O8 83.5(11) . . ?
O13 W2 O3 159.1(10) . . ?
O8A W2 O3 55.9(11) . . ?
O24A W2 O3 58.5(12) . . ?
O22 W2 O3 97.7(10) 10_657 . ?
O25 W2 O3 96.7(10) 10_657 . ?
O24 W2 O3 74.0(11) . . ?
O8 W2 O3 72.3(11) . . ?
O13 W2 O4 157.6(9) . 10_657 ?
O8A W2 O4 85.1(12) . 10_657 ?
O24A W2 O4 83.0(12) . 10_657 ?
O22 W2 O4 65.2(10) 10_657 10_657 ?
O25 W2 O4 68.3(9) 10_657 10_657 ?
O24 W2 O4 104.6(11) . 10_657 ?
O8 W2 O4 105.5(11) . 10_657 ?
O3 W2 O4 43.3(10) . 10_657 ?
O14 W3 O27 111.2(12) . . ?
O14 W3 O19 98.6(8) . . ?
O27 W3 O19 149.8(12) . . ?
O14 W3 O21 101.8(10) . 10_657 ?
O27 W3 O21 90.1(11) . 10_657 ?
O19 W3 O21 88.4(8) . 10_657 ?
O14 W3 O18 98.6(9) . . ?
O27 W3 O18 82.2(12) . . ?
O19 W3 O18 88.8(8) . . ?
O21 W3 O18 159.6(10) 10_657 . ?
O14 W3 O27A 90.1(11) . . ?
O27 W3 O27A 21.9(11) . . ?
O19 W3 O27A 171.2(11) . . ?
O21 W3 O27A 88.7(10) 10_657 . ?
O18 W3 O27A 91.0(11) . . ?
O14 W3 O2 158.7(9) . 10_657 ?
O27 W3 O2 55.9(13) . 10_657 ?
O19 W3 O2 96.9(9) . 10_657 ?
O21 W3 O2 64.1(10) 10_657 10_657 ?
O18 W3 O2 96.3(10) . 10_657 ?
O27A W3 O2 74.3(11) . 10_657 ?
O14 W3 O1 158.8(9) . . ?
O27 W3 O1 84.1(12) . . ?
O19 W3 O1 65.8(8) . . ?
O21 W3 O1 92.4(11) 10_657 . ?
O18 W3 O1 68.1(9) . . ?
O27A W3 O1 106.0(11) . . ?
O2 W3 O1 42.5(9) 10_657 . ?
O12 W4 O27 111.1(12) . 10_657 ?
O12 W4 O26 101.3(10) . . ?
O27 W4 O26 91.4(12) 10_657 . ?
O12 W4 O25 95.9(10) . . ?
O27 W4 O25 86.1(12) 10_657 . ?
O26 W4 O25 162.3(10) . . ?
O12 W4 O23 98.6(9) . . ?
O27 W4 O23 150.2(13) 10_657 . ?
O26 W4 O23 85.3(10) . . ?
O25 W4 O23 88.2(8) . . ?
O12 W4 O27A 90.3(11) . 10_657 ?
O27 W4 O27A 21.7(11) 10_657 10_657 ?
O26 W4 O27A 89.6(11) . 10_657 ?
O25 W4 O27A 94.3(11) . 10_657 ?
O23 W4 O27A 170.5(12) . 10_657 ?
O12 W4 O2 158.4(9) . . ?
O27 W4 O2 54.9(12) 10_657 . ?
O26 W4 O2 65.6(10) . . ?
O25 W4 O2 99.0(10) . . ?
O23 W4 O2 97.4(9) . . ?
O27A W4 O2 73.1(11) 10_657 . ?
O12 W4 O4 157.0(9) . . ?
O27 W4 O4 84.9(13) 10_657 . ?
O26 W4 O4 94.4(11) . . ?
O25 W4 O4 67.9(10) . . ?
O23 W4 O4 65.9(9) . . ?
O27A W4 O4 106.6(12) 10_657 . ?
O2 W4 O4 44.5(9) . . ?
O12 W4 K1 40.9(7) . . ?
O27 W4 K1 101.4(10) 10_657 . ?
O26 W4 K1 142.2(8) . . ?
O25 W4 K1 55.2(7) . . ?
O23 W4 K1 99.2(7) . . ?
O27A W4 K1 89.8(9) 10_657 . ?
O2 W4 K1 148.5(7) . . ?
O4 W4 K1 121.8(7) . . ?
O15 W5 O8A 110.7(12) . . ?
O15 W5 O18 98.4(10) . . ?
O8A W5 O18 84.8(11) . . ?
O15 W5 O28A 110.8(12) . . ?
O8A W5 O28A 91.8(12) . . ?
O18 W5 O28A 149.8(11) . . ?
O15 W5 O16 99.2(10) . . ?
O8A W5 O16 150.0(11) . . ?
O18 W5 O16 88.4(8) . . ?
O28A W5 O16 79.7(11) . . ?
O15 W5 O28 90.4(12) . . ?
O8A W5 O28 90.0(12) . . ?
O18 W5 O28 170.9(11) . . ?
O28A W5 O28 22.6(9) . . ?
O16 W5 O28 92.4(10) . . ?
O15 W5 O8 90.0(11) . . ?
O8A W5 O8 21.6(9) . . ?
O18 W5 O8 94.0(10) . . ?
O28A W5 O8 93.6(12) . . ?
O16 W5 O8 170.0(11) . . ?
O28 W5 O8 83.8(11) . . ?
O15 W5 O3 158.8(10) . . ?
O8A W5 O3 56.1(11) . . ?
O18 W5 O3 96.8(10) . . ?
O28A W5 O3 57.6(12) . . ?
O16 W5 O3 96.0(9) . . ?
O28 W5 O3 74.2(11) . . ?
O8 W5 O3 74.1(10) . . ?
O15 W5 O1 157.9(9) . . ?
O8A W5 O1 85.6(11) . . ?
O18 W5 O1 67.4(8) . . ?
O28A W5 O1 82.5(11) . . ?
O16 W5 O1 64.9(9) . . ?
O28 W5 O1 104.8(10) . . ?
O8 W5 O1 107.1(10) . . ?
O3 W5 O1 43.3(9) . . ?
O17 W6 O28A 111.5(12) . . ?
O17 W6 O24A 112.6(12) . . ?
O28A W6 O24A 94.5(14) . . ?
O17 W6 O21 99.6(10) . . ?
O28A W6 O21 148.2(12) . . ?
O24A W6 O21 78.8(13) . . ?
O17 W6 O26 98.7(10) . . ?
O28A W6 O26 79.4(12) . . ?
O24A W6 O26 148.1(13) . . ?
O21 W6 O26 90.0(9) . . ?
O17 W6 O24 94.2(11) . . ?
O28A W6 O24 91.8(12) . . ?
O24A W6 O24 21.2(11) . . ?
O21 W6 O24 92.1(10) . . ?
O26 W6 O24 166.4(12) . . ?
O17 W6 O28 92.9(10) . . ?
O28A W6 O28 21.9(10) . . ?
O24A W6 O28 91.6(13) . . ?
O21 W6 O28 166.5(11) . . ?
O26 W6 O28 93.3(11) . . ?
O24 W6 O28 81.7(11) . . ?
O17 W6 O2 154.5(9) . . ?
O28A W6 O2 85.3(12) . . ?
O24A W6 O2 83.8(13) . . ?
O21 W6 O2 63.2(9) . . ?
O26 W6 O2 64.6(10) . . ?
O24 W6 O2 104.6(11) . . ?
O28 W6 O2 106.6(10) . . ?
O17 W6 O3 159.1(9) . . ?
O28A W6 O3 55.8(12) . . ?
O24A W6 O3 57.3(12) . . ?
O21 W6 O3 96.0(11) . . ?
O26 W6 O3 95.0(10) . . ?
O24 W6 O3 71.4(10) . . ?
O28 W6 O3 70.6(11) . . ?
O2 W6 O3 46.3(9) . . ?
O5 Cu1 O10 162.4(7) . . ?
O5 Cu1 N2 90.2(7) . . ?
O10 Cu1 N2 89.2(7) . . ?
O5 Cu1 N4 89.2(8) . 12_547 ?
O10 Cu1 N4 91.0(7) . 12_547 ?
N2 Cu1 N4 178.4(8) . 12_547 ?
O5 Cu1 O1W 113.8(7) . . ?
O10 Cu1 O1W 83.8(6) . . ?
N2 Cu1 O1W 92.8(7) . . ?
N4 Cu1 O1W 88.8(7) 12_547 . ?
O5 Cu1 K1 148.2(5) . 5_545 ?
O10 Cu1 K1 46.1(4) . 5_545 ?
N2 Cu1 K1 69.5(5) . 5_545 ?
N4 Cu1 K1 111.8(6) 12_547 5_545 ?
O1W Cu1 K1 46.6(4) . 5_545 ?
O4W K2 O11 125(3) . 12_547 ?
O4W K2 N8 122(2) . . ?
O11 K2 N8 94.9(9) 12_547 . ?
O4W K2 O3W 109(3) . . ?
O11 K2 O3W 79.9(13) 12_547 . ?
N8 K2 O3W 119.0(15) . . ?
O4W K2 O5W 102(3) . . ?
O11 K2 O5W 126.8(14) 12_547 . ?
N8 K2 O5W 76.6(13) . . ?
O3W K2 O5W 61.1(15) . . ?
O4W K2 C2 144(3) . 12_547 ?
O11 K2 C2 19.1(9) 12_547 12_547 ?
N8 K2 C2 80.3(9) . 12_547 ?
O3W K2 C2 76.6(13) . 12_547 ?
O5W K2 C2 110.8(13) . 12_547 ?
O4W K2 C1 106(2) . . ?
O11 K2 C1 91.2(9) 12_547 . ?
N8 K2 C1 24.4(10) . . ?
O3W K2 C1 142.0(14) . . ?
O5W K2 C1 98.1(12) . . ?
C2 K2 C1 83.1(9) 12_547 . ?
O4W K2 O6W 60(3) . . ?
O11 K2 O6W 87.9(12) 12_547 . ?
N8 K2 O6W 84.9(14) . . ?
O3W K2 O6W 153.8(15) . . ?
O5W K2 O6W 141.4(14) . . ?
C2 K2 O6W 98.9(12) 12_547 . ?
C1 K2 O6W 60.6(13) . . ?
O4W K2 N10 126(2) . . ?
O11 K2 N10 101.0(9) 12_547 . ?
N8 K2 N10 16.6(10) . . ?
O3W K2 N10 104.6(13) . . ?
O5W K2 N10 60.6(11) . . ?
C2 K2 N10 83.6(8) 12_547 . ?
C1 K2 N10 40.7(9) . . ?
O6W K2 N10 100.5(12) . . ?
O4W K2 O7 167(3) . 12_547 ?
O11 K2 O7 42.7(8) 12_547 12_547 ?
N8 K2 O7 64.4(8) . 12_547 ?
O3W K2 O7 72.9(12) . 12_547 ?
O5W K2 O7 89.4(12) . 12_547 ?
C2 K2 O7 23.6(7) 12_547 12_547 ?
C1 K2 O7 75.6(9) . 12_547 ?
O6W K2 O7 112.7(12) . 12_547 ?
N10 K2 O7 63.2(7) . 12_547 ?
N8 Cu2 O5W 95.6(16) . . ?
N8 Cu2 O3W 161.3(17) . . ?
O5W Cu2 O3W 82.1(19) . . ?
N8 Cu2 O11 89.8(10) . 12_547 ?
O5W Cu2 O11 167.4(15) . 12_547 ?
O3W Cu2 O11 89.2(14) . 12_547 ?
N8 Cu2 O4W 94.7(18) . . ?
O5W Cu2 O4W 104(2) . . ?
O3W Cu2 O4W 104(2) . . ?
O11 Cu2 O4W 87.3(17) 12_547 . ?
O12 K1 O2W 145.4(7) . . ?
O12 K1 N6 123.2(6) . 9_654 ?
O2W K1 N6 70.4(9) . 9_654 ?
O12 K1 O1W 130.1(6) . 9_654 ?
O2W K1 O1W 83.4(7) . 9_654 ?
N6 K1 O1W 70.9(6) 9_654 9_654 ?
O12 K1 O6 96.0(6) . . ?
O2W K1 O6 57.3(8) . . ?
N6 K1 O6 125.8(6) 9_654 . ?
O1W K1 O6 113.1(6) 9_654 . ?
O12 K1 O10 85.6(5) . 9_654 ?
O2W K1 O10 125.2(7) . 9_654 ?
N6 K1 O10 61.2(6) 9_654 9_654 ?
O1W K1 O10 58.4(5) 9_654 9_654 ?
O6 K1 O10 168.4(5) . 9_654 ?
O12 K1 O14 67.4(5) . 18_546 ?
O2W K1 O14 93.1(8) . 18_546 ?
N6 K1 O14 69.9(6) 9_654 18_546 ?
O1W K1 O14 139.5(5) 9_654 18_546 ?
O6 K1 O14 98.1(5) . 18_546 ?
O10 K1 O14 93.1(5) 9_654 18_546 ?
O12 K1 N12 102.1(6) . . ?
O2W K1 N12 81.6(8) . . ?
N6 K1 N12 132.0(7) 9_654 . ?
O1W K1 N12 67.6(6) 9_654 . ?
O6 K1 N12 56.0(5) . . ?
O10 K1 N12 112.5(5) 9_654 . ?
O14 K1 N12 152.0(6) 18_546 . ?
O12 K1 O25 52.2(5) . . ?
O2W K1 O25 143.4(8) . . ?
N6 K1 O25 135.0(6) 9_654 . ?
O1W K1 O25 83.2(6) 9_654 . ?
O6 K1 O25 97.9(6) . . ?
O10 K1 O25 74.0(5) 9_654 . ?
O14 K1 O25 118.6(6) 18_546 . ?
N12 K1 O25 61.8(5) . . ?
O12 K1 W4 23.1(3) . . ?
O2W K1 W4 153.4(7) . . ?
N6 K1 W4 134.9(5) 9_654 . ?
O1W K1 W4 110.5(4) 9_654 . ?
O6 K1 W4 96.1(4) . . ?
O10 K1 W4 80.8(3) 9_654 . ?
O14 K1 W4 90.2(4) 18_546 . ?
N12 K1 W4 83.1(4) . . ?
O25 K1 W4 29.2(4) . . ?
O12 K1 Cu1 114.6(4) . 9_654 ?
O2W K1 Cu1 98.1(6) . 9_654 ?
N6 K1 Cu1 48.8(4) 9_654 9_654 ?
O1W K1 Cu1 34.5(4) 9_654 9_654 ?
O6 K1 Cu1 145.7(5) . 9_654 ?
O10 K1 Cu1 29.3(3) 9_654 9_654 ?
O14 K1 Cu1 107.5(4) 18_546 9_654 ?
N12 K1 Cu1 100.5(4) . 9_654 ?
O25 K1 Cu1 89.6(4) . 9_654 ?
W4 K1 Cu1 105.97(16) . 9_654 ?
B1 O1 O4 56.5(13) . . ?
B1 O1 O2 58.1(12) . 10_657 ?
O4 O1 O2 93.8(19) . 10_657 ?
B1 O1 O3 57.1(13) . . ?
O4 O1 O3 94.8(17) . . ?
O2 O1 O3 91.9(17) 10_657 . ?
B1 O1 W1 126.9(14) . . ?
O4 O1 W1 70.5(13) . . ?
O2 O1 W1 134.5(17) 10_657 . ?
O3 O1 W1 130.7(16) . . ?
B1 O1 W3 124.1(13) . . ?
O4 O1 W3 132.4(18) . . ?
O2 O1 W3 66.0(11) 10_657 . ?
O3 O1 W3 126.8(15) . . ?
W1 O1 W3 93.0(8) . . ?
B1 O1 W5 120.8(15) . . ?
O4 O1 W5 132.5(16) . . ?
O2 O1 W5 126.4(16) 10_657 . ?
O3 O1 W5 63.7(13) . . ?
W1 O1 W5 91.6(8) . . ?
W3 O1 W5 90.6(8) . . ?
B1 O2 O1 53.4(12) . 10_657 ?
B1 O2 W3 124.8(15) . 10_657 ?
O1 O2 W3 71.5(12) 10_657 10_657 ?
B1 O2 W4 121.2(13) . . ?
O1 O2 W4 134.2(18) 10_657 . ?
W3 O2 W4 94.9(10) 10_657 . ?
B1 O2 W6 120.5(15) . . ?
O1 O2 W6 130.2(17) 10_657 . ?
W3 O2 W6 94.4(9) 10_657 . ?
W4 O2 W6 93.4(10) . . ?
B1 O3 O4 52.9(14) . 10_657 ?
B1 O3 O1 52.4(12) . . ?
O4 O3 O1 89.4(18) 10_657 . ?
B1 O3 W5 125.4(14) . . ?
O4 O3 W5 135.7(17) 10_657 . ?
O1 O3 W5 73.0(13) . . ?
B1 O3 W2 122.3(16) . . ?
O4 O3 W2 69.4(13) 10_657 . ?
O1 O3 W2 136.5(16) . . ?
W5 O3 W2 95.7(9) . . ?
B1 O3 W6 118.8(13) . . ?
O4 O3 W6 126.7(16) 10_657 . ?
O1 O3 W6 129.5(16) . . ?
W5 O3 W6 94.3(11) . . ?
W2 O3 W6 92.5(9) . . ?
B1 O4 O1 56.2(13) . . ?
B1 O4 O3 57.4(12) . 10_657 ?
O1 O4 O3 94.4(17) . 10_657 ?
B1 O4 W2 124.6(15) . 10_657 ?
O1 O4 W2 131.6(18) . 10_657 ?
O3 O4 W2 67.3(13) 10_657 10_657 ?
B1 O4 W1 125.1(16) . . ?
O1 O4 W1 69.0(13) . . ?
O3 O4 W1 136.2(17) 10_657 . ?
W2 O4 W1 93.2(10) 10_657 . ?
B1 O4 W4 121.3(16) . . ?
O1 O4 W4 131.8(18) . . ?
O3 O4 W4 125.9(17) 10_657 . ?
W2 O4 W4 91.6(9) 10_657 . ?
W1 O4 W4 91.8(9) . . ?
C7 O5 Cu1 123.9(17) . . ?
C8 O6 K1 127.9(16) . . ?
C2 O7 K2 59.5(16) . 11_667 ?
O8A O8 W5 69(3) . . ?
O8A O8 W2 57(3) . . ?
W5 O8 W2 117.9(15) . . ?
O8 O8A W2 103(4) . . ?
O8 O8A W5 90(4) . . ?
W2 O8A W5 146.9(17) . . ?
C8 O10 Cu1 109.2(13) . . ?
C8 O10 K1 133.4(14) . 5_545 ?
Cu1 O10 K1 104.6(6) . 5_545 ?
C2 O11 K2 131(2) . 11_667 ?
C2 O11 Cu2 109(2) . 11_667 ?
K2 O11 Cu2 25.9(5) 11_667 11_667 ?
W4 O12 K1 116.0(9) . . ?
W3 O14 K1 156.5(9) . 17_556 ?
W1 O16 W5 135.6(12) . . ?
W5 O18 W3 133.7(11) . . ?
W3 O19 W1 133.8(11) . . ?
W6 O21 W3 137.7(12) . 10_657 ?
W1 O22 W2 135.5(14) . 10_657 ?
W1 O23 W4 134.7(13) . . ?
O24A O24 W2 70(4) . . ?
O24A O24 W6 62(4) . . ?
W2 O24 W6 121.6(16) . . ?
O24 O24A W6 97(4) . . ?
O24 O24A W2 88(4) . . ?
W6 O24A W2 145.7(18) . . ?
W4 O25 W2 132.1(12) . 10_657 ?
W4 O25 K1 95.6(8) . . ?
W2 O25 K1 130.3(10) 10_657 . ?
W4 O26 W6 135.8(14) . . ?
O27A O27 W3 96(4) . . ?
O27A O27 W4 97(4) . 10_657 ?
W3 O27 W4 149(2) . 10_657 ?
O27 O27A W3 62(3) . . ?
O27 O27A W4 61(3) . 10_657 ?
W3 O27A W4 117.6(16) . 10_657 ?
O28A O28 W5 71(3) . . ?
O28A O28 W6 60(3) . . ?
W5 O28 W6 120.7(15) . . ?
O28 O28A W6 98(3) . . ?
O28 O28A W5 86(3) . . ?
W6 O28A W5 145.1(17) . . ?
Cu1 O1W K1 99.0(6) . 5_545 ?
C1 N1 N12 109(2) . . ?
C1 N1 C9 130(2) . . ?
N12 N1 C9 121(2) . . ?
C5 N2 N6 105.7(19) . . ?
C5 N2 Cu1 131.9(16) . . ?
N6 N2 Cu1 122.4(14) . . ?
C3 N3 N9 107(2) . . ?
C3 N3 C4 133(2) . . ?
N9 N3 C4 120(2) . . ?
C3 N4 N11 102(2) . . ?
C3 N4 Cu1 135.9(18) . 11_667 ?
N11 N4 Cu1 121.9(17) . 11_667 ?
C5 N5 N7 106.1(18) . . ?
C5 N5 C6 131.7(19) . . ?
N7 N5 C6 122(2) . . ?
N7 N6 N2 112(2) . . ?
N7 N6 K1 127.2(16) . 5_545 ?
N2 N6 K1 118.0(15) . 5_545 ?
N6 N7 N5 107(2) . . ?
C1 N8 N10 104(3) . . ?
C1 N8 Cu2 142(3) . . ?
N10 N8 Cu2 114(2) . . ?
C1 N8 K2 117(2) . . ?
N10 N8 K2 138(2) . . ?
N11 N9 N3 107(3) . . ?
N12 N10 N8 113(3) . . ?
N12 N10 K2 138(2) . . ?
N8 N10 K2 25.2(13) . . ?
N9 N11 N4 111(2) . . ?
N10 N12 N1 105(2) . . ?
N10 N12 K1 124.9(19) . . ?
N1 N12 K1 130.5(15) . . ?
N1 C1 N8 109(3) . . ?
N1 C1 K2 148(2) . . ?
N8 C1 K2 38.8(17) . . ?
O11 C2 O7 126(3) . . ?
O11 C2 C6 116(3) . . ?
O7 C2 C6 118(3) . . ?
O11 C2 K2 29.5(13) . 11_667 ?
O7 C2 K2 96.9(18) . 11_667 ?
C6 C2 K2 145(2) . 11_667 ?
N4 C3 N3 114(2) . . ?
N3 C4 C7 115(2) . . ?
N2 C5 N5 109.0(18) . . ?
N5 C6 C2 114(2) . . ?
O9 C7 O5 122(3) . . ?
O9 C7 C4 121(3) . . ?
O5 C7 C4 117(2) . . ?
O6 C8 O10 122(2) . . ?
O6 C8 C9 124(2) . . ?
O10 C8 C9 114(2) . . ?
N1 C9 C8 112(2) . . ?

_refine_diff_density_max         2.064
_refine_diff_density_min         -1.873
_refine_diff_density_rms         0.313

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_SiWCu
_database_code_depnum_ccdc_archive 'CCDC 2069056'
loop_
_audit_author_name
_audit_author_address
'Shenzhen Chang'
;Dalian University of Technology
China
;
_audit_update_record             
;
2021-06-15 deposited with the CCDC.	2021-09-29 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2018/3
_shelx_SHELXL_version_number     2018/3
_chemical_name_systematic        SiWCu
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C18 H67 Cu3 K3 N24 O76 Si W12'
_chemical_formula_weight         4378.16

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      trigonal
_space_group_IT_number           147
_space_group_name_H-M_alt        'P -3'
_space_group_name_Hall           '-P 3'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'

_cell_length_a                   15.570(3)
_cell_length_b                   15.570(3)
_cell_length_c                   10.337(3)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     2170.3(11)
_cell_formula_units_Z            1
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    2548
_cell_measurement_theta_min      2.483
_cell_measurement_theta_max      24.992

_exptl_crystal_description       block
_exptl_crystal_colour            blue
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    3.350
_exptl_crystal_F_000             1997
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.250
_exptl_crystal_size_mid          0.240
_exptl_crystal_size_min          0.230
_exptl_absorpt_coefficient_mu    16.836
_shelx_estimated_absorpt_T_min   0.102
_shelx_estimated_absorpt_T_max   0.113
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.021
_exptl_absorpt_correction_T_max  0.021
_exptl_absorpt_process_details   'ABSCOR by T.Higashi 8 March, 1995'
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker Smart Apex CCD'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            11390
_diffrn_reflns_av_unetI/netI     0.0341
_diffrn_reflns_av_R_equivalents  0.0457
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_theta_min         2.483
_diffrn_reflns_theta_max         24.992
_diffrn_reflns_theta_full        24.992
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measured_fraction_theta_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_point_group_measured_fraction_full 0.996
_reflns_number_total             2548
_reflns_number_gt                2353
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          
;
Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0701P)²+41.4034P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_extinction_coef       0.0038(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         2548
_refine_ls_number_parameters     233
_refine_ls_number_restraints     36
_refine_ls_R_factor_all          0.0475
_refine_ls_R_factor_gt           0.0445
_refine_ls_wR_factor_ref         0.1284
_refine_ls_wR_factor_gt          0.1258
_refine_ls_goodness_of_fit_ref   1.075
_refine_ls_restrained_S_all      1.084
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.94588(3) 0.85086(3) 0.21983(4) 0.0268(2) Uani 1 1 d . . . . .
W2 W 1.04116(4) 0.79713(4) 0.49934(5) 0.0359(2) Uani 1 1 d . . . . .
O3 O 0.8395(12) 0.7915(15) 0.3406(16) 0.024(4) Uani 0.5 1 d . . P A 1
O3A O 0.8205(16) 0.7439(15) 0.3004(18) 0.035(5) Uani 0.5 1 d . . P A 2
O4 O 1.0081(15) 0.7794(15) 0.3013(18) 0.032(4) Uani 0.5 1 d . . P A 3
O4A O 1.0207(13) 0.8243(15) 0.3388(16) 0.024(4) Uani 0.5 1 d . . P A 4
O5 O 0.9198(8) 0.7774(9) 0.0911(11) 0.062(3) Uani 1 1 d . . . . .
O6 O 1.0718(7) 0.9605(7) 0.1747(13) 0.057(3) Uani 1 1 d . . . . .
O7 O 0.8947(13) 0.7097(14) 0.5162(17) 0.028(4) Uani 0.5 1 d . U P A 5
O7A O 0.9126(14) 0.7572(14) 0.5482(16) 0.026(4) Uani 0.5 1 d . . P A 6
O8 O 1.0597(10) 0.6994(8) 0.5002(10) 0.058(3) Uani 1 1 d . . . . .
O9 O 0.0023(12) 0.3994(11) 1.1452(16) 0.087(4) Uani 1 1 d . U . . .
O10 O 0.1154(14) 0.4570(12) 1.0227(15) 0.094(4) Uani 1 1 d . U . . .
O1W O 0.569(2) 0.423(2) 1.214(3) 0.193(12) Uani 1 1 d . U . . .
OW1 O 0.666667 0.333333 1.066(4) 0.129(12) Uiso 1 3 d S . P . .
OW2 O 1.0180(15) 0.5093(15) 0.5568(17) 0.114(6) Uiso 1 1 d . . . . .
OW3 O 0.788(3) 0.564(3) 1.253(4) 0.232(15) Uiso 1 1 d . . . . .
N1 N 0.2352(11) 0.4134(10) 1.1772(14) 0.061(4) Uani 1 1 d . . . . .
N2 N 0.2864(17) 0.4029(16) 1.083(2) 0.107(6) Uani 1 1 d . U . . .
N3 N 0.396(2) 0.458(2) 1.135(3) 0.056(7) Uani 0.5 1 d . . P B 7
N3A N 0.3695(16) 0.4815(19) 1.076(3) 0.047(6) Uani 0.5 1 d . . P B 8
N4 N 0.3755(17) 0.5212(17) 1.204(2) 0.109(7) Uani 1 1 d . U . . .
C1 C 0.0789(19) 0.4106(12) 1.1147(17) 0.066(5) Uani 1 1 d . . . . .
C2 C 0.1273(11) 0.3632(11) 1.1886(16) 0.051(4) Uani 1 1 d . . . . .
H2A H 0.110208 0.360588 1.279302 0.061 Uiso 1 1 calc R U . . .
H2B H 0.099970 0.295408 1.158666 0.061 Uiso 1 1 calc R U . . .
C3 C 0.2943(11) 0.4902(13) 1.2481(16) 0.063(5) Uani 1 1 d . . . . .
H3A H 0.276793 0.515536 1.318391 0.076 Uiso 1 1 calc R U . . .
O2 O 0.9596(11) 0.8875(11) 0.4421(14) 0.079(4) Uani 1 1 d . . . . .
O1 O 1.000000 1.000000 0.345(2) 0.076(6) Uani 1 3 d S T P A .
Si1 Si 1.000000 1.000000 0.500000 0.0167(13) Uani 1 6 d S T P . .
K1 K 0.5192(2) 0.4807(2) 1.0511(3) 0.0719(8) Uani 0.5 1 d . . P B .
Cu1 Cu 0.5192(2) 0.4807(2) 1.0511(3) 0.0719(8) Uani 0.5 1 d . . P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 O5 1.667(9) . ?
W1 O4A 1.876(16) . ?
W1 O6 1.879(9) 3_675 ?
W1 O3 1.904(15) . ?
W1 O6 1.905(10) . ?
W1 O4 1.991(18) . ?
W1 O3A 2.01(2) . ?
W1 O2 2.351(14) . ?
W1 O1 2.414(13) . ?
W2 O8 1.685(9) . ?
W2 O3 1.765(15) 6_656 ?
W2 O4A 1.781(16) . ?
W2 O7A 1.845(17) . ?
W2 O7A 1.854(17) 6_656 ?
W2 O7 1.987(18) 6_656 ?
W2 O7 1.995(18) . ?
W2 O4 2.095(19) . ?
W2 O3A 2.126(19) 6_656 ?
W2 O2 2.394(15) . ?
W2 O2 2.403(15) 6_656 ?
O9 C1 1.16(3) . ?
O9 K1 1.939(14) 3_565 ?
O9 K1 2.620(15) 6_557 ?
O10 C1 1.16(2) . ?
O10 K1 2.028(16) 6_557 ?
O10 K1 2.617(18) 3_565 ?
O1W K1 2.22(3) . ?
OW2 OW2 1.27(3) 4_766 ?
N1 C3 1.31(2) . ?
N1 N2 1.32(2) . ?
N1 C2 1.46(2) . ?
N2 N3A 1.26(3) . ?
N2 N3 1.58(4) . ?
N2 K1 2.98(2) 4_667 ?
N2 K1 3.21(2) . ?
N3 N4 1.38(4) . ?
N3 K1 1.96(3) . ?
N3 K1 2.26(3) 4_667 ?
N3A N4 1.44(3) . ?
N3A K1 2.01(2) 4_667 ?
N3A K1 2.35(3) . ?
N4 C3 1.20(2) . ?
N4 K1 3.05(2) . ?
N4 K1 3.11(2) 4_667 ?
C1 C2 1.50(2) . ?
C1 K1 2.64(2) 3_565 ?
C1 K1 2.694(17) 6_557 ?
C2 H2A 0.9700 . ?
C2 H2B 0.9700 . ?
C3 H3A 0.9300 . ?
O2 Si1 1.650(15) . ?
O1 Si1 1.60(2) . ?
K1 K1 1.482(7) 4_667 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 W1 O4A 109.7(7) . . ?
O5 W1 O6 102.1(6) . 3_675 ?
O4A W1 O6 148.1(7) . 3_675 ?
O5 W1 O3 109.6(8) . . ?
O6 W1 O3 84.2(6) 3_675 . ?
O5 W1 O6 102.0(6) . . ?
O4A W1 O6 83.3(7) . . ?
O6 W1 O6 88.3(6) 3_675 . ?
O3 W1 O6 148.4(8) . . ?
O5 W1 O4 88.5(7) . . ?
O6 W1 O4 169.1(7) 3_675 . ?
O6 W1 O4 91.9(7) . . ?
O5 W1 O3A 87.7(7) . . ?
O6 W1 O3A 93.4(7) 3_675 . ?
O6 W1 O3A 169.6(7) . . ?
O5 W1 O2 155.2(6) . . ?
O4A W1 O2 54.7(7) . . ?
O6 W1 O2 95.8(5) 3_675 . ?
O3 W1 O2 55.1(7) . . ?
O6 W1 O2 95.4(5) . . ?
O4 W1 O2 73.3(6) . . ?
O3A W1 O2 74.2(7) . . ?
O5 W1 O1 159.6(7) . . ?
O4A W1 O1 84.4(7) . . ?
O6 W1 O1 64.3(5) 3_675 . ?
O3 W1 O1 85.1(8) . . ?
O6 W1 O1 64.0(5) . . ?
O4 W1 O1 106.1(7) . . ?
O3A W1 O1 107.6(7) . . ?
O2 W1 O1 45.2(6) . . ?
O8 W2 O3 109.1(8) . 6_656 ?
O8 W2 O4A 110.6(7) . . ?
O8 W2 O7A 110.0(7) . . ?
O8 W2 O7A 111.2(7) . 6_656 ?
O3 W2 O7A 92.1(7) 6_656 6_656 ?
O8 W2 O7 93.1(7) . 6_656 ?
O3 W2 O7 87.5(7) 6_656 6_656 ?
O4A W2 O7 90.6(8) . 6_656 ?
O7A W2 O7 153.9(9) . 6_656 ?
O7A W2 O7 21.5(5) 6_656 6_656 ?
O8 W2 O7 92.1(7) . . ?
O7 W2 O7 174.8(10) 6_656 . ?
O8 W2 O4 91.6(6) . . ?
O8 W2 O3A 90.1(7) . 6_656 ?
O3 W2 O3A 20.2(7) 6_656 6_656 ?
O4A W2 O3A 158.3(9) . 6_656 ?
O7A W2 O3A 86.3(8) . 6_656 ?
O7A W2 O3A 92.9(8) 6_656 6_656 ?
O7 W2 O3A 81.4(8) 6_656 6_656 ?
O7 W2 O3A 98.2(8) . 6_656 ?
O4 W2 O3A 178.0(8) . 6_656 ?
O8 W2 O2 155.9(5) . . ?
O3 W2 O2 87.9(8) 6_656 . ?
O4A W2 O2 54.5(7) . . ?
O7A W2 O2 57.3(6) . . ?
O7A W2 O2 84.2(7) 6_656 . ?
O7 W2 O2 104.9(7) 6_656 . ?
O7 W2 O2 70.2(6) . . ?
O4 W2 O2 70.6(6) . . ?
O3A W2 O2 108.0(6) 6_656 . ?
O8 W2 O2 156.1(6) . 6_656 ?
O3 W2 O2 55.1(7) 6_656 6_656 ?
O2 W2 O2 47.9(6) . 6_656 ?
W2 O3 W1 149.9(10) 5_566 . ?
W1 O3A W2 118.0(10) . 5_566 ?
W1 O4 W2 119.7(9) . . ?
W2 O4A W1 150.2(10) . . ?
W1 O6 W1 137.4(7) 2_765 . ?
W2 O7 W2 124.5(10) 5_566 . ?
W2 O7A W2 144.5(9) . 5_566 ?
C1 O9 K1 114.4(14) . 3_565 ?
C1 O9 K1 81.0(12) . 6_557 ?
K1 O9 K1 33.9(3) 3_565 6_557 ?
C1 O10 K1 112.7(17) . 6_557 ?
C1 O10 K1 78.4(15) . 3_565 ?
K1 O10 K1 34.3(3) 6_557 3_565 ?
C3 N1 N2 109.5(15) . . ?
C3 N1 C2 122.6(14) . . ?
N2 N1 C2 126.7(17) . . ?
N3A N2 N1 108(2) . . ?
N1 N2 N3 103.9(19) . . ?
N3A N2 K1 31.5(13) . 4_667 ?
N1 N2 K1 139.6(14) . 4_667 ?
N3 N2 K1 48.1(13) . 4_667 ?
N3A N2 K1 38.0(16) . . ?
N1 N2 K1 131.9(15) . . ?
N3 N2 K1 28.0(12) . . ?
K1 N2 K1 27.3(2) 4_667 . ?
N4 N3 N2 89(2) . . ?
N4 N3 K1 131(2) . . ?
N2 N3 K1 129.9(19) . . ?
N4 N3 K1 115(2) . 4_667 ?
N2 N3 K1 100.5(17) . 4_667 ?
K1 N3 K1 40.3(6) . 4_667 ?
N2 N3A N4 100(2) . . ?
N2 N3A K1 129.4(18) . 4_667 ?
N4 N3A K1 127.7(16) . 4_667 ?
N2 N3A K1 123(2) . . ?
N4 N3A K1 104.6(18) . . ?
K1 N3A K1 38.7(5) 4_667 . ?
C3 N4 N3 119(2) . . ?
C3 N4 N3A 110(2) . . ?
C3 N4 K1 148.4(17) . . ?
N3 N4 K1 29.2(14) . . ?
N3A N4 K1 48.3(13) . . ?
C3 N4 K1 141.0(16) . 4_667 ?
N3 N4 K1 41.0(15) . 4_667 ?
N3A N4 K1 30.8(10) . 4_667 ?
K1 N4 K1 27.8(2) . 4_667 ?
O10 C1 O9 118(2) . . ?
O10 C1 C2 121(2) . . ?
O9 C1 C2 121.2(18) . . ?
O10 C1 K1 76.2(13) . 3_565 ?
O9 C1 K1 42.0(10) . 3_565 ?
C2 C1 K1 162.2(15) . 3_565 ?
O10 C1 K1 44.0(12) . 6_557 ?
O9 C1 K1 73.9(12) . 6_557 ?
C2 C1 K1 164.8(16) . 6_557 ?
K1 C1 K1 32.2(3) 3_565 6_557 ?
N1 C2 C1 114.9(15) . . ?
N1 C2 H2A 108.5 . . ?
C1 C2 H2A 108.5 . . ?
N1 C2 H2B 108.5 . . ?
C1 C2 H2B 108.5 . . ?
H2A C2 H2B 107.5 . . ?
N4 C3 N1 105.8(16) . . ?
N4 C3 H3A 127.1 . . ?
N1 C3 H3A 127.1 . . ?
Si1 O2 W1 123.5(8) . . ?
Si1 O2 W2 120.1(7) . . ?
W1 O2 W2 96.3(5) . . ?
Si1 O2 W2 119.6(8) . 5_566 ?
W1 O2 W2 96.4(5) . 5_566 ?
W2 O2 W2 94.5(5) . 5_566 ?
Si1 O1 W1 122.5(5) . . ?
Si1 O1 W1 122.5(5) . 3_675 ?
W1 O1 W1 93.8(7) . 3_675 ?
Si1 O1 W1 122.5(5) . 2_765 ?
W1 O1 W1 93.8(7) . 2_765 ?
W1 O1 W1 93.8(7) 3_675 2_765 ?
O1 Si1 O1 180.0 . 4_776 ?
O1 Si1 O2 111.3(5) . 4_776 ?
O1 Si1 O2 68.7(5) 4_776 4_776 ?
O1 Si1 O2 111.3(5) . 5_566 ?
O1 Si1 O2 68.7(5) 4_776 5_566 ?
O2 Si1 O2 107.6(5) 4_776 5_566 ?
O1 Si1 O2 68.7(5) . 2_765 ?
O1 Si1 O2 111.3(5) 4_776 2_765 ?
O2 Si1 O2 72.4(5) 4_776 2_765 ?
O2 Si1 O2 180.0 5_566 2_765 ?
O1 Si1 O2 111.3(5) . 6_656 ?
O1 Si1 O2 68.7(5) 4_776 6_656 ?
O2 Si1 O2 107.6(5) 4_776 6_656 ?
O2 Si1 O2 107.6(5) 5_566 6_656 ?
O2 Si1 O2 72.4(5) 2_765 6_656 ?
O1 Si1 O2 68.7(5) . 3_675 ?
O1 Si1 O2 111.3(5) 4_776 3_675 ?
O2 Si1 O2 72.4(5) 4_776 3_675 ?
O2 Si1 O2 72.4(5) 5_566 3_675 ?
O2 Si1 O2 107.6(5) 2_765 3_675 ?
O2 Si1 O2 180.0 6_656 3_675 ?
O1 Si1 O2 68.7(5) . . ?
O1 Si1 O2 111.3(5) 4_776 . ?
O2 Si1 O2 180.0 4_776 . ?
O2 Si1 O2 72.4(5) 5_566 . ?
O2 Si1 O2 107.6(5) 2_765 . ?
O2 Si1 O2 72.4(5) 6_656 . ?
O2 Si1 O2 107.6(5) 3_675 . ?
K1 K1 O9 99.1(6) 4_667 2_665 ?
K1 K1 N3 80.5(10) 4_667 . ?
O9 K1 N3 93.2(9) 2_665 . ?
K1 K1 N3A 83.0(10) 4_667 4_667 ?
O9 K1 N3A 89.8(8) 2_665 4_667 ?
K1 K1 O10 95.2(6) 4_667 5_557 ?
O9 K1 O10 164.9(7) 2_665 5_557 ?
K1 K1 O1W 175.8(9) 4_667 . ?
O9 K1 O1W 80.0(10) 2_665 . ?
N3 K1 O1W 95.4(13) . . ?
N3A K1 O1W 101.0(13) 4_667 . ?
O10 K1 O1W 86.1(10) 5_557 . ?
K1 K1 N3 59.1(8) 4_667 4_667 ?
O9 K1 N3 93.2(9) 2_665 4_667 ?
O10 K1 N3 89.8(9) 5_557 4_667 ?
O1W K1 N3 124.9(12) . 4_667 ?
K1 K1 N3A 58.3(8) 4_667 . ?
O9 K1 N3A 95.9(7) 2_665 . ?
N3A K1 N3A 141.3(5) 4_667 . ?
O10 K1 N3A 95.8(8) 5_557 . ?
O1W K1 N3A 117.7(12) . . ?
K1 K1 O10 50.5(4) 4_667 2_665 ?
O9 K1 O10 48.8(6) 2_665 2_665 ?
O10 K1 O10 145.7(3) 5_557 2_665 ?
O1W K1 O10 128.1(9) . 2_665 ?
K1 K1 O9 46.9(4) 4_667 5_557 ?
O9 K1 O9 146.1(3) 2_665 5_557 ?
O10 K1 O9 48.5(6) 5_557 5_557 ?
O1W K1 O9 133.8(9) . 5_557 ?
O10 K1 O9 97.3(5) 2_665 5_557 ?
K1 K1 C1 75.9(5) 4_667 2_665 ?
O9 K1 C1 23.6(6) 2_665 2_665 ?
O10 K1 C1 171.1(7) 5_557 2_665 ?
O1W K1 C1 102.8(10) . 2_665 ?
O10 K1 C1 25.4(5) 2_665 2_665 ?
O9 K1 C1 122.7(5) 5_557 2_665 ?
K1 K1 C1 71.8(6) 4_667 5_557 ?
O9 K1 C1 170.1(7) 2_665 5_557 ?
O10 K1 C1 23.3(7) 5_557 5_557 ?
O1W K1 C1 109.3(10) . 5_557 ?
O10 K1 C1 122.4(6) 2_665 5_557 ?
O9 K1 C1 25.2(5) 5_557 5_557 ?
C1 K1 C1 147.8(3) 2_665 5_557 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O8 W2 O4A W1 131(2) . . . . ?
O2 W2 O4A W1 -28(2) . . . . ?
O2 W2 O4A W1 -66(3) 6_656 . . . ?
O5 W1 O4A W2 -130(2) . . . . ?
O6 W1 O4A W2 54(3) 3_675 . . . ?
O6 W1 O4A W2 130(3) . . . . ?
O2 W1 O4A W2 28(2) . . . . ?
O1 W1 O4A W2 65(3) . . . . ?
O8 W2 O7A W2 -125.5(18) . . . 5_566 ?
O7A W2 O7A W2 55.4(18) 6_656 . . 5_566 ?
O2 W2 O7A W2 31.6(16) . . . 5_566 ?
O2 W2 O7A W2 74.3(19) 6_656 . . 5_566 ?
C3 N1 N2 N3A -14(3) . . . . ?
C2 N1 N2 N3A 154(2) . . . . ?
C3 N1 N2 N3 23(2) . . . . ?
C2 N1 N2 N3 -169.4(18) . . . . ?
C3 N1 N2 K1 -17(3) . . . 4_667 ?
C2 N1 N2 K1 150.9(17) . . . 4_667 ?
C3 N1 N2 K1 21(3) . . . . ?
C2 N1 N2 K1 -171.1(12) . . . . ?
N1 N2 N3 N4 -30(2) . . . . ?
K1 N2 N3 N4 116(2) 4_667 . . . ?
K1 N2 N3 N4 147(4) . . . . ?
N1 N2 N3 K1 -177(2) . . . . ?
K1 N2 N3 K1 -31.2(16) 4_667 . . . ?
N1 N2 N3 K1 -146.2(16) . . . 4_667 ?
K1 N2 N3 K1 31.2(16) . . . 4_667 ?
N1 N2 N3A N4 21(3) . . . . ?
K1 N2 N3A N4 -163(5) 4_667 . . . ?
K1 N2 N3A N4 -115(3) . . . . ?
N1 N2 N3A K1 -176(2) . . . 4_667 ?
K1 N2 N3A K1 47.7(18) . . . 4_667 ?
N1 N2 N3A K1 136.1(19) . . . . ?
K1 N2 N3A K1 -47.7(18) 4_667 . . . ?
N2 N3 N4 C3 34(3) . . . . ?
K1 N3 N4 C3 -179(2) . . . . ?
K1 N3 N4 C3 135(2) 4_667 . . . ?
N2 N3 N4 K1 -146(4) . . . . ?
K1 N3 N4 K1 -45.2(19) 4_667 . . . ?
N2 N3 N4 K1 -101(2) . . . 4_667 ?
K1 N3 N4 K1 45.2(19) . . . 4_667 ?
N2 N3A N4 C3 -24(3) . . . . ?
K1 N3A N4 C3 173(2) 4_667 . . . ?
K1 N3A N4 C3 -152(2) . . . . ?
N2 N3A N4 K1 128(3) . . . . ?
K1 N3A N4 K1 -35.1(16) 4_667 . . . ?
N2 N3A N4 K1 163(4) . . . 4_667 ?
K1 N3A N4 K1 35.1(16) . . . 4_667 ?
K1 O10 C1 O9 6(2) 6_557 . . . ?
K1 O10 C1 O9 7.0(16) 3_565 . . . ?
K1 O10 C1 C2 -176.5(12) 6_557 . . . ?
K1 O10 C1 C2 -175.5(16) 3_565 . . . ?
K1 O10 C1 K1 -1.0(8) 6_557 . . 3_565 ?
K1 O10 C1 K1 1.0(8) 3_565 . . 6_557 ?
K1 O9 C1 O10 -10(2) 3_565 . . . ?
K1 O9 C1 O10 -4.4(17) 6_557 . . . ?
K1 O9 C1 C2 172.3(12) 3_565 . . . ?
K1 O9 C1 C2 178.1(16) 6_557 . . . ?
K1 O9 C1 K1 5.9(9) 6_557 . . 3_565 ?
K1 O9 C1 K1 -5.9(9) 3_565 . . 6_557 ?
C3 N1 C2 C1 83(2) . . . . ?
N2 N1 C2 C1 -83(2) . . . . ?
O10 C1 C2 N1 27(2) . . . . ?
O9 C1 C2 N1 -155.5(18) . . . . ?
K1 C1 C2 N1 -138(4) 3_565 . . . ?
K1 C1 C2 N1 18(5) 6_557 . . . ?
N3 N4 C3 N1 -25(3) . . . . ?
N3A N4 C3 N1 16(3) . . . . ?
K1 N4 C3 N1 -25(4) . . . . ?
K1 N4 C3 N1 22(4) 4_667 . . . ?
N2 N1 C3 N4 -3(3) . . . . ?
C2 N1 C3 N4 -171.0(19) . . . . ?
W1 O1 Si1 O2 -179.8(5) . . . 4_776 ?
W1 O1 Si1 O2 -59.8(5) 3_675 . . 4_776 ?
W1 O1 Si1 O2 60.2(5) 2_765 . . 4_776 ?
W1 O1 Si1 O2 -59.8(5) . . . 5_566 ?
W1 O1 Si1 O2 60.2(5) 3_675 . . 5_566 ?
W1 O1 Si1 O2 -179.8(5) 2_765 . . 5_566 ?
W1 O1 Si1 O2 120.2(5) . . . 2_765 ?
W1 O1 Si1 O2 -119.8(5) 3_675 . . 2_765 ?
W1 O1 Si1 O2 0.2(5) 2_765 . . 2_765 ?
W1 O1 Si1 O2 60.2(5) . . . 6_656 ?
W1 O1 Si1 O2 -179.8(5) 3_675 . . 6_656 ?
W1 O1 Si1 O2 -59.8(5) 2_765 . . 6_656 ?
W1 O1 Si1 O2 -119.8(5) . . . 3_675 ?
W1 O1 Si1 O2 0.2(5) 3_675 . . 3_675 ?
W1 O1 Si1 O2 120.2(5) 2_765 . . 3_675 ?
W1 O1 Si1 O2 0.2(5) . . . . ?
W1 O1 Si1 O2 120.2(5) 3_675 . . . ?
W1 O1 Si1 O2 -119.8(5) 2_765 . . . ?
W1 O2 Si1 O1 -0.2(6) . . . . ?
W2 O2 Si1 O1 122.2(8) . . . . ?
W2 O2 Si1 O1 -122.2(8) 5_566 . . . ?
W1 O2 Si1 O1 179.8(6) . . . 4_776 ?
W2 O2 Si1 O1 -57.8(8) . . . 4_776 ?
W2 O2 Si1 O1 57.8(8) 5_566 . . 4_776 ?
W1 O2 Si1 O2 121.9(8) . . . 5_566 ?
W2 O2 Si1 O2 -115.7(13) . . . 5_566 ?
W2 O2 Si1 O2 0.0(6) 5_566 . . 5_566 ?
W1 O2 Si1 O2 -58.1(8) . . . 2_765 ?
W2 O2 Si1 O2 64.3(13) . . . 2_765 ?
W2 O2 Si1 O2 -180.0(6) 5_566 . . 2_765 ?
W1 O2 Si1 O2 -122.4(8) . . . 6_656 ?
W2 O2 Si1 O2 0.0(6) . . . 6_656 ?
W2 O2 Si1 O2 115.7(13) 5_566 . . 6_656 ?
W1 O2 Si1 O2 57.6(8) . . . 3_675 ?
W2 O2 Si1 O2 -180.0(6) . . . 3_675 ?
W2 O2 Si1 O2 -64.3(13) 5_566 . . 3_675 ?

_refine_diff_density_max         2.126
_refine_diff_density_min         -2.791
_refine_diff_density_rms         0.367

